#------------------------------------------------------------------------------
#$Date: 2015-06-04 14:34:11 +0300 (Thu, 04 Jun 2015) $
#$Revision: 137956 $
#$URL: svn://www.crystallography.net/cod/cif/4/34/32/4343231.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4343231
loop_
_publ_author_name
'Read, Cory Michael'
'Smith, Mark D.'
'Withers, Ray'
'Zur Loye, Hans-Conrad'
_publ_section_title
;
 Flux Crystal Growth and Optical Properties of Two Uranium-Containing
 Silicates: A2USiO6 (A = Cs, Rb).
;
_journal_issue                   9
_journal_name_full               'Inorganic chemistry'
_journal_page_first              4520
_journal_page_last               4525
_journal_paper_doi               10.1021/acs.inorgchem.5b00364
_journal_volume                  54
_journal_year                    2015
_chemical_formula_moiety         'Cs2 O6 Si U'
_chemical_formula_sum            'Cs2 O6 Si U'
_chemical_formula_weight         627.94
_chemical_name_systematic
; 
 ? 
;
_space_group_crystal_system      orthorhombic
_space_group_IT_number           71
_space_group_name_Hall           '-I 2 2'
_space_group_name_H-M_alt        'I m m m'
_symmetry_space_group_name_Hall  '-I 2 2'
_symmetry_space_group_name_H-M   'I m m m'
_audit_creation_method           SHELXL-2013
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.5812(4)
_cell_length_b                   13.0011(6)
_cell_length_c                   13.8811(7)
_cell_measurement_reflns_used    2813
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      32.556
_cell_measurement_theta_min      2.935
_cell_volume                     1548.65(13)
_computing_cell_refinement       'SAINT-Plus Version 6.45 (Bruker, 2001)'
_computing_data_collection       'SMART Version 5.625 (Bruker, 2001)'
_computing_data_reduction        'SAINT-Plus Version 6.45 (Bruker, 2001)'
_computing_molecular_graphics    various
_computing_publication_material  various
_computing_structure_refinement  'SHELXL-2013 (Sheldrick, 2013)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.983
_diffrn_measurement_device_type  'Bruker SMART APEX CCD diffractometer'
_diffrn_measurement_method       'omega and phi scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0561
_diffrn_reflns_av_unetI/netI     0.0283
_diffrn_reflns_laue_measured_fraction_full 0.999
_diffrn_reflns_laue_measured_fraction_max 0.983
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            16331
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.983
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         32.570
_diffrn_reflns_theta_min         2.146
_diffrn_source                   'sealed tube'
_exptl_absorpt_coefficient_mu    30.357
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.4161
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS Version 2.05 (Bruker, 2001)'
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    5.386
_exptl_crystal_description       needle
_exptl_crystal_F_000             2112
_exptl_crystal_size_max          0.100
_exptl_crystal_size_mid          0.040
_exptl_crystal_size_min          0.030
_refine_diff_density_max         1.564
_refine_diff_density_min         -2.277
_refine_diff_density_rms         0.299
_refine_ls_extinction_coef       0.00059(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.052
_refine_ls_matrix_type           full
_refine_ls_number_parameters     62
_refine_ls_number_reflns         1576
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.052
_refine_ls_R_factor_all          0.0327
_refine_ls_R_factor_gt           0.0253
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
; 
 w=1/[σ²(Fo²)+(0.0219P)²+5.0845P] 
 where P=(Fo²+2Fc²)/3 
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0506
_refine_ls_wR_factor_ref         0.0531
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1358
_reflns_number_total             1576
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            ic5b00364_si_002.cif
_cod_data_source_block           Cs2USiO6
_cod_database_code               4343231
_shelx_estimated_absorpt_t_min   0.151
_shelx_estimated_absorpt_t_max   0.463
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'x, -y, -z'
'-x, y, -z'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z'
'-x, y, z'
'x, -y, z'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'-x+1/2, y+1/2, z+1/2'
'x+1/2, -y+1/2, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
U1 U 0.2500 0.2500 0.2500 0.00877(7) Uani 1 2 d S . P
Cs1 Cs 0.0000 0.5000 0.15534(5) 0.02222(14) Uani 1 4 d S T P
Cs2 Cs 0.0000 0.0000 0.30534(5) 0.01927(14) Uani 1 4 d S T P
Cs3 Cs 0.0000 0.26498(5) 0.5000 0.01996(14) Uani 1 4 d S T P
Cs4 Cs 0.0000 0.19171(5) 0.0000 0.02081(14) Uani 1 4 d S T P
Si1 Si 0.18953(18) 0.5000 0.38806(12) 0.0087(3) Uani 1 2 d S T P
O1 O 0.2442(3) 0.3271(3) 0.1371(3) 0.0190(7) Uani 1 1 d . . .
O2 O 0.2512(3) 0.3973(3) 0.3373(3) 0.0210(8) Uani 1 1 d . . .
O3 O 0.0000 0.2471(3) 0.2537(4) 0.0238(13) Uani 1 2 d S T P
O4 O 0.0000 0.5000 0.3896(5) 0.0182(14) Uani 1 4 d S T P
O5 O 0.2479(7) 0.5000 0.5000 0.0199(15) Uani 1 4 d S T P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 U1 O1 180.0 . 13
O1 U1 O3 90.18(17) . .
O1 U1 O3 89.81(17) 13 .
O1 U1 O3 89.81(17) . 13
O1 U1 O3 90.19(17) 13 13
O3 U1 O3 180.0(2) . 13
O1 U1 O2 90.30(14) . 13
O1 U1 O2 89.70(14) 13 13
O3 U1 O2 89.61(14) . 13
O3 U1 O2 90.39(14) 13 13
O1 U1 O2 89.71(14) . .
O1 U1 O2 90.30(14) 13 .
O3 U1 O2 90.39(14) . .
O3 U1 O2 89.61(14) 13 .
O2 U1 O2 180.0 13 .
O1 U1 Cs2 126.14(11) . .
O1 U1 Cs2 53.86(11) 13 .
O3 U1 Cs2 55.98(12) . .
O3 U1 Cs2 124.02(12) 13 .
O2 U1 Cs2 53.78(9) 13 .
O2 U1 Cs2 126.22(9) . .
O1 U1 Cs2 53.86(11) . 13
O1 U1 Cs2 126.14(11) 13 13
O3 U1 Cs2 124.02(12) . 13
O3 U1 Cs2 55.98(12) 13 13
O2 U1 Cs2 126.22(9) 13 13
O2 U1 Cs2 53.78(9) . 13
Cs2 U1 Cs2 180.0 . 13
O1 U1 Cs3 47.50(10) . 13
O1 U1 Cs3 132.50(10) 13 13
O3 U1 Cs3 123.00(14) . 13
O3 U1 Cs3 57.00(14) 13 13
O2 U1 Cs3 60.52(9) 13 13
O2 U1 Cs3 119.48(9) . 13
Cs2 U1 Cs3 114.158(11) . 13
Cs2 U1 Cs3 65.842(11) 13 13
O1 U1 Cs3 132.50(10) . .
O1 U1 Cs3 47.50(10) 13 .
O3 U1 Cs3 57.00(14) . .
O3 U1 Cs3 123.00(14) 13 .
O2 U1 Cs3 119.48(9) 13 .
O2 U1 Cs3 60.52(9) . .
Cs2 U1 Cs3 65.843(11) . .
Cs2 U1 Cs3 114.158(11) 13 .
Cs3 U1 Cs3 180.0 13 .
O1 U1 Cs1 44.82(10) . .
O1 U1 Cs1 135.18(10) 13 .
O3 U1 Cs1 60.00(13) . .
O3 U1 Cs1 120.00(13) 13 .
O2 U1 Cs1 119.67(9) 13 .
O2 U1 Cs1 60.33(9) . .
Cs2 U1 Cs1 115.296(4) . .
Cs2 U1 Cs1 64.704(4) 13 .
Cs3 U1 Cs1 92.306(11) 13 .
Cs3 U1 Cs1 87.694(11) . .
O1 U1 Cs1 135.18(10) . 13
O1 U1 Cs1 44.82(10) 13 13
O3 U1 Cs1 120.00(13) . 13
O3 U1 Cs1 60.00(13) 13 13
O2 U1 Cs1 60.33(9) 13 13
O2 U1 Cs1 119.67(9) . 13
Cs2 U1 Cs1 64.704(4) . 13
Cs2 U1 Cs1 115.296(4) 13 13
Cs3 U1 Cs1 87.694(11) 13 13
Cs3 U1 Cs1 92.306(11) . 13
Cs1 U1 Cs1 180.0 . 13
O1 Cs1 O1 170.60(14) 11 12_565
O1 Cs1 O1 93.59(12) 11 2_565
O1 Cs1 O1 85.64(12) 12_565 2_565
O1 Cs1 O1 85.64(12) 11 .
O1 Cs1 O1 93.59(12) 12_565 .
O1 Cs1 O1 170.60(14) 2_565 .
O1 Cs1 O4 94.70(7) 11 .
O1 Cs1 O4 94.70(7) 12_565 .
O1 Cs1 O4 94.70(7) 2_565 .
O1 Cs1 O4 94.70(7) . .
O1 Cs1 O3 50.08(7) 11 .
O1 Cs1 O3 134.80(7) 12_565 .
O1 Cs1 O3 134.80(7) 2_565 .
O1 Cs1 O3 50.08(7) . .
O4 Cs1 O3 67.45(8) . .
O1 Cs1 O3 134.80(7) 11 2_565
O1 Cs1 O3 50.08(7) 12_565 2_565
O1 Cs1 O3 50.08(7) 2_565 2_565
O1 Cs1 O3 134.80(7) . 2_565
O4 Cs1 O3 67.45(8) . 2_565
O3 Cs1 O3 134.89(16) . 2_565
O1 Cs1 O2 137.67(9) 11 12_565
O1 Cs1 O2 51.42(9) 12_565 12_565
O1 Cs1 O2 101.25(8) 2_565 12_565
O1 Cs1 O2 85.44(8) . 12_565
O4 Cs1 O2 45.12(5) . 12_565
O3 Cs1 O2 94.25(8) . 12_565
O3 Cs1 O2 52.03(8) 2_565 12_565
O1 Cs1 O2 51.42(9) 11 11
O1 Cs1 O2 137.67(9) 12_565 11
O1 Cs1 O2 85.44(8) 2_565 11
O1 Cs1 O2 101.25(8) . 11
O4 Cs1 O2 45.12(5) . 11
O3 Cs1 O2 52.03(8) . 11
O3 Cs1 O2 94.25(8) 2_565 11
O2 Cs1 O2 90.24(11) 12_565 11
O1 Cs1 O2 85.44(8) 11 2_565
O1 Cs1 O2 101.25(8) 12_565 2_565
O1 Cs1 O2 51.42(9) 2_565 2_565
O1 Cs1 O2 137.67(9) . 2_565
O4 Cs1 O2 45.12(5) . 2_565
O3 Cs1 O2 94.25(8) . 2_565
O3 Cs1 O2 52.03(8) 2_565 2_565
O2 Cs1 O2 74.08(11) 12_565 2_565
O2 Cs1 O2 43.83(11) 11 2_565
O1 Cs1 O2 101.25(8) 11 .
O1 Cs1 O2 85.44(8) 12_565 .
O1 Cs1 O2 137.67(9) 2_565 .
O1 Cs1 O2 51.42(9) . .
O4 Cs1 O2 45.12(5) . .
O3 Cs1 O2 52.02(8) . .
O3 Cs1 O2 94.25(8) 2_565 .
O2 Cs1 O2 43.83(11) 12_565 .
O2 Cs1 O2 74.07(11) 11 .
O2 Cs1 O2 90.24(11) 2_565 .
O1 Cs1 Si1 76.56(7) 11 2_565
O1 Cs1 Si1 112.26(7) 12_565 2_565
O1 Cs1 Si1 76.56(7) 2_565 2_565
O1 Cs1 Si1 112.26(7) . 2_565
O4 Cs1 Si1 26.72(3) . 2_565
O3 Cs1 Si1 69.97(7) . 2_565
O3 Cs1 Si1 69.97(7) 2_565 2_565
O2 Cs1 Si1 68.94(6) 12_565 2_565
O2 Cs1 Si1 25.70(5) 11 2_565
O2 Cs1 Si1 25.70(5) 2_565 2_565
O2 Cs1 Si1 68.94(6) . 2_565
O2 Cs2 O2 49.29(12) 14_445 7_455
O2 Cs2 O2 103.66(13) 14_445 13
O2 Cs2 O2 83.59(12) 7_455 13
O2 Cs2 O2 83.59(13) 14_445 8_545
O2 Cs2 O2 103.66(13) 7_455 8_545
O2 Cs2 O2 49.29(12) 13 8_545
O2 Cs2 O1 153.21(9) 14_445 13
O2 Cs2 O1 108.33(8) 7_455 13
O2 Cs2 O1 53.97(9) 13 13
O2 Cs2 O1 89.43(8) 8_545 13
O2 Cs2 O1 53.97(9) 14_445 14_445
O2 Cs2 O1 89.43(8) 7_455 14_445
O2 Cs2 O1 153.21(9) 13 14_445
O2 Cs2 O1 108.33(8) 8_545 14_445
O1 Cs2 O1 151.48(13) 13 14_445
O2 Cs2 O1 108.33(8) 14_445 8_545
O2 Cs2 O1 153.21(9) 7_455 8_545
O2 Cs2 O1 89.43(8) 13 8_545
O2 Cs2 O1 53.97(9) 8_545 8_545
O1 Cs2 O1 87.80(12) 13 8_545
O1 Cs2 O1 85.25(11) 14_445 8_545
O2 Cs2 O1 89.43(8) 14_445 7_455
O2 Cs2 O1 53.97(9) 7_455 7_455
O2 Cs2 O1 108.33(8) 13 7_455
O2 Cs2 O1 153.21(9) 8_545 7_455
O1 Cs2 O1 85.25(11) 13 7_455
O1 Cs2 O1 87.80(12) 14_445 7_455
O1 Cs2 O1 151.48(13) 8_545 7_455
O2 Cs2 O3 57.21(8) 14_445 2
O2 Cs2 O3 105.81(9) 7_455 2
O2 Cs2 O3 105.81(9) 13 2
O2 Cs2 O3 57.21(8) 8_545 2
O1 Cs2 O3 136.92(6) 13 2
O1 Cs2 O3 51.45(7) 14_445 2
O1 Cs2 O3 51.45(7) 8_545 2
O1 Cs2 O3 136.92(6) 7_455 2
O2 Cs2 O3 105.81(9) 14_445 .
O2 Cs2 O3 57.21(8) 7_455 .
O2 Cs2 O3 57.21(8) 13 .
O2 Cs2 O3 105.81(9) 8_545 .
O1 Cs2 O3 51.45(7) 13 .
O1 Cs2 O3 136.92(6) 14_445 .
O1 Cs2 O3 136.92(6) 8_545 .
O1 Cs2 O3 51.45(7) 7_455 .
O3 Cs2 O3 154.85(18) 2 .
O2 Cs2 Si1 24.75(6) 14_445 14_445
O2 Cs2 Si1 24.75(6) 7_455 14_445
O2 Cs2 Si1 91.77(7) 13 14_445
O2 Cs2 Si1 91.77(7) 8_545 14_445
O1 Cs2 Si1 130.68(6) 13 14_445
O1 Cs2 Si1 72.41(6) 14_445 14_445
O1 Cs2 Si1 130.68(6) 8_545 14_445
O1 Cs2 Si1 72.41(6) 7_455 14_445
O3 Cs2 Si1 81.11(6) 2 14_445
O3 Cs2 Si1 81.11(6) . 14_445
O2 Cs2 Si1 91.77(7) 14_445 13
O2 Cs2 Si1 91.77(7) 7_455 13
O2 Cs2 Si1 24.75(6) 13 13
O2 Cs2 Si1 24.75(6) 8_545 13
O1 Cs2 Si1 72.41(6) 13 13
O1 Cs2 Si1 130.68(6) 14_445 13
O1 Cs2 Si1 72.41(6) 8_545 13
O1 Cs2 Si1 130.68(6) 7_455 13
O3 Cs2 Si1 81.11(6) 2 13
O3 Cs2 Si1 81.11(6) . 13
Si1 Cs2 Si1 89.56(5) 14_445 13
O1 Cs3 O1 135.20(13) 7_455 6
O1 Cs3 O1 74.57(13) 7_455 16_455
O1 Cs3 O1 88.60(12) 6 16_455
O1 Cs3 O1 88.60(12) 7_455 13
O1 Cs3 O1 74.57(13) 6 13
O1 Cs3 O1 135.20(13) 16_455 13
O1 Cs3 O4 127.75(8) 7_455 9_566
O1 Cs3 O4 93.96(10) 6 9_566
O1 Cs3 O4 93.96(10) 16_455 9_566
O1 Cs3 O4 127.75(8) 13 9_566
O1 Cs3 O4 93.96(10) 7_455 .
O1 Cs3 O4 127.75(8) 6 .
O1 Cs3 O4 127.75(8) 16_455 .
O1 Cs3 O4 93.96(10) 13 .
O4 Cs3 O4 53.3(2) 9_566 .
O1 Cs3 O3 125.34(8) 7_455 10_556
O1 Cs3 O3 50.93(7) 6 10_556
O1 Cs3 O3 50.93(7) 16_455 10_556
O1 Cs3 O3 125.34(8) 13 10_556
O4 Cs3 O3 67.27(12) 9_566 10_556
O4 Cs3 O3 120.53(13) . 10_556
O1 Cs3 O3 50.93(7) 7_455 .
O1 Cs3 O3 125.34(8) 6 .
O1 Cs3 O3 125.34(8) 16_455 .
O1 Cs3 O3 50.93(7) 13 .
O4 Cs3 O3 120.53(13) 9_566 .
O4 Cs3 O3 67.27(12) . .
O3 Cs3 O3 172.20(16) 10_556 .
O1 Cs3 O2 102.85(9) 7_455 .
O1 Cs3 O2 98.36(8) 6 .
O1 Cs3 O2 171.92(9) 16_455 .
O1 Cs3 O2 51.51(8) 13 .
O4 Cs3 O2 81.53(10) 9_566 .
O4 Cs3 O2 44.33(7) . .
O3 Cs3 O2 131.68(7) 10_556 .
O3 Cs3 O2 53.17(7) . .
O1 Cs3 O2 171.92(9) 7_455 10_556
O1 Cs3 O2 51.51(8) 6 10_556
O1 Cs3 O2 102.85(9) 16_455 10_556
O1 Cs3 O2 98.36(8) 13 10_556
O4 Cs3 O2 44.33(7) 9_566 10_556
O4 Cs3 O2 81.53(10) . 10_556
O3 Cs3 O2 53.17(7) 10_556 10_556
O3 Cs3 O2 131.68(7) . 10_556
O2 Cs3 O2 78.64(11) . 10_556
O1 Cs3 O2 51.51(8) 7_455 11
O1 Cs3 O2 171.92(9) 6 11
O1 Cs3 O2 98.36(8) 16_455 11
O1 Cs3 O2 102.85(9) 13 11
O4 Cs3 O2 81.53(10) 9_566 11
O4 Cs3 O2 44.33(7) . 11
O3 Cs3 O2 131.68(7) 10_556 11
O3 Cs3 O2 53.17(7) . 11
O2 Cs3 O2 74.42(11) . 11
O2 Cs3 O2 122.31(11) 10_556 11
O1 Cs3 O2 98.36(8) 7_455 4_556
O1 Cs3 O2 102.85(9) 6 4_556
O1 Cs3 O2 51.51(8) 16_455 4_556
O1 Cs3 O2 171.92(9) 13 4_556
O4 Cs3 O2 44.33(7) 9_566 4_556
O4 Cs3 O2 81.53(10) . 4_556
O3 Cs3 O2 53.17(7) 10_556 4_556
O3 Cs3 O2 131.68(7) . 4_556
O2 Cs3 O2 122.31(11) . 4_556
O2 Cs3 O2 74.42(11) 10_556 4_556
O2 Cs3 O2 78.64(11) 11 4_556
O5 Cs4 O5 81.91(15) 5_444 13
O5 Cs4 O2 46.73(6) 5_444 16_454
O5 Cs4 O2 99.12(8) 13 16_454
O5 Cs4 O2 99.12(8) 5_444 13
O5 Cs4 O2 46.73(6) 13 13
O2 Cs4 O2 139.17(12) 16_454 13
O5 Cs4 O2 46.73(6) 5_444 7_455
O5 Cs4 O2 99.12(8) 13 7_455
O2 Cs4 O2 85.86(12) 16_454 7_455
O2 Cs4 O2 80.14(12) 13 7_455
O5 Cs4 O2 99.12(8) 5_444 6_554
O5 Cs4 O2 46.73(6) 13 6_554
O2 Cs4 O2 80.14(12) 16_454 6_554
O2 Cs4 O2 85.86(12) 13 6_554
O2 Cs4 O2 139.17(12) 7_455 6_554
O5 Cs4 O1 144.18(6) 5_444 .
O5 Cs4 O1 89.24(8) 13 .
O2 Cs4 O1 167.89(9) 16_454 .
O2 Cs4 O1 52.46(8) 13 .
O2 Cs4 O1 101.53(8) 7_455 .
O2 Cs4 O1 99.70(8) 6_554 .
O5 Cs4 O1 89.24(8) 5_444 4
O5 Cs4 O1 144.18(6) 13 4
O2 Cs4 O1 52.46(8) 16_454 4
O2 Cs4 O1 167.89(9) 13 4
O2 Cs4 O1 99.70(8) 7_455 4
O2 Cs4 O1 101.53(8) 6_554 4
O1 Cs4 O1 116.25(12) . 4
O5 Cs4 O1 144.18(6) 5_444 10
O5 Cs4 O1 89.24(8) 13 10
O2 Cs4 O1 101.53(8) 16_454 10
O2 Cs4 O1 99.70(8) 13 10
O2 Cs4 O1 167.89(9) 7_455 10
O2 Cs4 O1 52.46(8) 6_554 10
O1 Cs4 O1 69.64(12) . 10
O1 Cs4 O1 77.89(11) 4 10
O5 Cs4 O1 89.24(8) 5_444 11
O5 Cs4 O1 144.18(6) 13 11
O2 Cs4 O1 99.70(8) 16_454 11
O2 Cs4 O1 101.53(8) 13 11
O2 Cs4 O1 52.46(8) 7_455 11
O2 Cs4 O1 167.89(9) 6_554 11
O1 Cs4 O1 77.89(11) . 11
O1 Cs4 O1 69.64(12) 4 11
O1 Cs4 O1 116.25(12) 10 11
O5 Cs4 O3 98.70(6) 5_444 .
O5 Cs4 O3 98.70(6) 13 .
O2 Cs4 O3 137.49(6) 16_454 .
O2 Cs4 O3 53.31(7) 13 .
O2 Cs4 O3 53.31(7) 7_455 .
O2 Cs4 O3 137.49(6) 6_554 .
O1 Cs4 O3 48.31(7) . .
O1 Cs4 O3 116.98(8) 4 .
O1 Cs4 O3 116.98(8) 10 .
O1 Cs4 O3 48.31(7) 11 .
O5 Cs4 O3 98.70(6) 5_444 10
O5 Cs4 O3 98.70(6) 13 10
O2 Cs4 O3 53.31(7) 16_454 10
O2 Cs4 O3 137.49(6) 13 10
O2 Cs4 O3 137.49(6) 7_455 10
O2 Cs4 O3 53.31(7) 6_554 10
O1 Cs4 O3 116.98(8) . 10
O1 Cs4 O3 48.31(7) 4 10
O1 Cs4 O3 48.31(7) 10 10
O1 Cs4 O3 116.98(8) 11 10
O3 Cs4 O3 156.91(15) . 10
O2 Si1 O2 113.2(3) . 12_565
O2 Si1 O4 109.67(17) . .
O2 Si1 O4 109.67(17) 12_565 .
O2 Si1 O5 108.53(18) . .
O2 Si1 O5 108.53(18) 12_565 .
O4 Si1 O5 107.1(3) . .
O2 Si1 Cs1 75.83(15) . .
O2 Si1 Cs1 75.83(15) 12_565 .
O4 Si1 Cs1 64.0(2) . .
O5 Si1 Cs1 171.1(2) . .
O2 Si1 Cs2 56.93(14) . 13
O2 Si1 Cs2 56.93(14) 12_565 13
O4 Si1 Cs2 135.6(2) . 13
O5 Si1 Cs2 117.4(2) . 13
Cs1 Si1 Cs2 71.51(3) . 13
O2 Si1 Cs3 69.51(13) . .
O2 Si1 Cs3 173.88(14) 12_565 .
O4 Si1 Cs3 64.27(11) . .
O5 Si1 Cs3 75.03(11) . .
Cs1 Si1 Cs3 99.96(3) . .
Cs2 Si1 Cs3 126.34(2) 13 .
O2 Si1 Cs3 173.88(14) . 9_566
O2 Si1 Cs3 69.52(13) 12_565 9_566
O4 Si1 Cs3 64.27(11) . 9_566
O5 Si1 Cs3 75.03(11) . 9_566
Cs1 Si1 Cs3 99.96(3) . 9_566
Cs2 Si1 Cs3 126.34(2) 13 9_566
Cs3 Si1 Cs3 107.28(4) . 9_566
O2 Si1 Cs4 118.36(13) . 5
O2 Si1 Cs4 54.96(14) 12_565 5
O4 Si1 Cs4 131.80(13) . 5
O5 Si1 Cs4 54.61(13) . 5
Cs1 Si1 Cs4 130.70(3) . 5
Cs2 Si1 Cs4 78.75(3) 13 5
Cs3 Si1 Cs4 129.32(4) . 5
Cs3 Si1 Cs4 67.749(16) 9_566 5
O2 Si1 Cs4 54.96(14) . 13
O2 Si1 Cs4 118.36(13) 12_565 13
O4 Si1 Cs4 131.80(13) . 13
O5 Si1 Cs4 54.61(13) . 13
Cs1 Si1 Cs4 130.70(3) . 13
Cs2 Si1 Cs4 78.75(3) 13 13
Cs3 Si1 Cs4 67.749(16) . 13
Cs3 Si1 Cs4 129.32(4) 9_566 13
Cs4 Si1 Cs4 77.89(3) 5 13
U1 O1 Cs1 110.00(14) . .
U1 O1 Cs3 106.62(13) . 13
Cs1 O1 Cs3 143.33(13) . 13
U1 O1 Cs2 98.53(13) . 13
Cs1 O1 Cs2 86.25(9) . 13
Cs3 O1 Cs2 86.59(8) 13 13
U1 O1 Cs4 102.29(13) . .
Cs1 O1 Cs4 90.26(8) . .
Cs3 O1 Cs4 83.79(9) 13 .
Cs2 O1 Cs4 158.82(12) 13 .
Si1 O2 U1 159.9(2) . .
Si1 O2 Cs2 98.31(16) . 13
U1 O2 Cs2 91.43(11) . 13
Si1 O2 Cs4 101.77(17) . 13
U1 O2 Cs4 94.15(11) . 13
Cs2 O2 Cs4 97.89(8) 13 13
Si1 O2 Cs3 85.61(14) . .
U1 O2 Cs3 85.89(10) . .
Cs2 O2 Cs3 174.76(11) 13 .
Cs4 O2 Cs3 77.84(8) 13 .
Si1 O2 Cs1 78.47(14) . .
U1 O2 Cs1 86.29(11) . .
Cs2 O2 Cs1 79.03(9) 13 .
Cs4 O2 Cs1 176.91(12) 13 .
Cs3 O2 Cs1 105.25(8) . .
U1 O3 U1 176.6(3) 7_455 .
U1 O3 Cs2 91.30(12) 7_455 .
U1 O3 Cs2 91.30(12) . .
U1 O3 Cs3 91.31(14) 7_455 .
U1 O3 Cs3 91.31(14) . .
Cs2 O3 Cs3 81.33(11) . .
U1 O3 Cs1 88.53(13) 7_455 .
U1 O3 Cs1 88.53(13) . .
Cs2 O3 Cs1 170.02(17) . .
Cs3 O3 Cs1 108.65(12) . .
U1 O3 Cs4 88.85(14) 7_455 .
U1 O3 Cs4 88.85(14) . .
Cs2 O3 Cs4 91.03(11) . .
Cs3 O3 Cs4 172.35(15) . .
Cs1 O3 Cs4 78.99(11) . .
Si1 O4 Si1 178.5(5) 2_565 .
Si1 O4 Cs1 89.2(2) 2_565 .
Si1 O4 Cs1 89.2(2) . .
Si1 O4 Cs3 90.35(11) 2_565 .
Si1 O4 Cs3 90.34(11) . .
Cs1 O4 Cs3 116.63(10) . .
Si1 O4 Cs3 90.35(11) 2_565 9_566
Si1 O4 Cs3 90.34(11) . 9_566
Cs1 O4 Cs3 116.63(10) . 9_566
Cs3 O4 Cs3 126.7(2) . 9_566
Si1 O5 Si1 144.3(4) . 10_556
Si1 O5 Cs4 101.60(11) . 5
Si1 O5 Cs4 101.60(11) 10_556 5
Si1 O5 Cs4 101.60(11) . 13
Si1 O5 Cs4 101.60(11) 10_556 13
Cs4 O5 Cs4 98.09(15) 5 13
Si1 O5 Cs3 79.90(13) . .
Si1 O5 Cs3 79.90(13) 10_556 .
Cs4 O5 Cs3 173.89(15) 5 .
Cs4 O5 Cs3 75.802(10) 13 .
Si1 O5 Cs3 79.90(13) . 9_566
Si1 O5 Cs3 79.90(13) 10_556 9_566
Cs4 O5 Cs3 75.802(10) 5 9_566
Cs4 O5 Cs3 173.89(15) 13 9_566
Cs3 O5 Cs3 110.31(15) . 9_566
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
U1 O1 1.861(4) .
U1 O1 1.861(4) 13
U1 O3 2.14626(19) .
U1 O3 2.1463(2) 13
U1 O2 2.266(3) 13
U1 O2 2.266(3) .
U1 Cs2 3.96947(19) .
U1 Cs2 3.96948(18) 13
U1 Cs3 4.08449(16) 13
U1 Cs3 4.08449(16) .
U1 Cs1 4.1101(2) .
U1 Cs1 4.1101(3) 13
Cs1 O1 3.083(3) 11
Cs1 O1 3.083(3) 12_565
Cs1 O1 3.083(3) 2_565
Cs1 O1 3.083(3) .
Cs1 O4 3.252(7) .
Cs1 O3 3.561(5) .
Cs1 O3 3.561(5) 2_565
Cs1 O2 3.579(4) 12_565
Cs1 O2 3.579(4) 11
Cs1 O2 3.579(4) 2_565
Cs1 O2 3.579(4) .
Cs1 Si1 3.6166(18) 2_565
Cs2 O2 3.203(4) 14_445
Cs2 O2 3.203(4) 7_455
Cs2 O2 3.203(4) 13
Cs2 O2 3.203(4) 8_545
Cs2 O1 3.241(3) 13
Cs2 O1 3.241(3) 14_445
Cs2 O1 3.241(3) 8_545
Cs2 O1 3.241(3) 7_455
Cs2 O3 3.291(5) 2
Cs2 O3 3.291(5) .
Cs2 Si1 3.7822(17) 14_445
Cs2 Si1 3.7822(17) 13
Cs3 O1 3.143(3) 7_455
Cs3 O1 3.143(3) 6
Cs3 O1 3.143(3) 16_455
Cs3 O1 3.143(3) 13
Cs3 O4 3.418(3) 9_566
Cs3 O4 3.418(3) .
Cs3 O3 3.426(5) 10_556
Cs3 O3 3.426(5) .
Cs3 O2 3.565(4) .
Cs3 O2 3.565(4) 10_556
Cs3 O2 3.565(4) 11
Cs3 O2 3.565(4) 4_556
Cs4 O5 3.300(4) 5_444
Cs4 O5 3.300(4) 13
Cs4 O2 3.316(4) 16_454
Cs4 O2 3.316(4) 13
Cs4 O2 3.316(4) 7_455
Cs4 O2 3.316(4) 6_554
Cs4 O1 3.334(3) .
Cs4 O1 3.334(3) 4
Cs4 O1 3.334(3) 10
Cs4 O1 3.334(3) 11
Cs4 O3 3.595(5) .
Cs4 O3 3.595(5) 10
Si1 O2 1.600(3) .
Si1 O2 1.600(3) 12_565
Si1 O4 1.6265(16) .
Si1 O5 1.633(2) .
Si1 Cs2 3.7822(17) 13
Si1 Cs3 3.7942(11) 9_566
Si1 Cs4 3.9655(13) 5
Si1 Cs4 3.9655(13) 13
O1 Cs3 3.143(3) 13
O1 Cs2 3.241(3) 13
O2 Cs2 3.203(4) 13
O2 Cs4 3.316(4) 13
O3 U1 2.14626(19) 7_455
O4 Si1 1.6265(16) 2_565
O4 Cs3 3.418(3) 9_566
O5 Si1 1.633(2) 10_556
O5 Cs4 3.300(4) 5
O5 Cs4 3.300(4) 13
O5 Cs3 3.723(3) 9_566
